**SIMULATION OF DELAMINATION IN ** **COMPOSITES UNDER QUASI-STATIC AND ** **FATIGUE LOADING USING COHESIVE ZONE **

**MODELS **

**Albert TURON TRAVESA **

**ISBN: 978-84-690-4372-1 **
**Dipòsit legal: GI-285-2007**

Escola Polit`ecnica Superior

Dept. d’Enginyeria Mec`anica i de la Construcci´o Industrial

## Simulation of delamination in composites under quasi-static

## and fatigue loading using cohesive zone models

A thesis submitted for the degree of Doctor of Philosophy by

### Albert Turon Travesa

2006

Advisors:

Pedro P. Camanho Josep Costa Balanzat

*Universidade do Porto, Portugal* *Universitat de Girona, Spain*

Dr. Pedro P. Camanho, Assistant Professor at the University of Porto, and Josep Costa Balanzat, Associate Professor at the University of Girona,

CERTIFY that the study entitled “Simulation of delamination in composites under quasi-static and fatigue loading using cohesive zone models” has been carried out under their supervision by Albert Turon Travesa to obtain the doctoral degree,

Girona, October 2006,

Pedro P. Camanho Josep Costa Balanzat

*Universidade do Porto, Portugal* *Universitat de Girona, Spain*

grant BR01/09. Also, it has been partially funded by the Spanish Government under research projects MAT2000–00741–C02–01 and MAT2003–09768–C03–01.

This research was conducted in part during the author’s visits to the Universidade do Porto, Portugal, and NASA Langley Research Center, Hampton VA, USA, which were funded by University of Girona and by NASA Langley Research Center.

## Agra¨ıments - Aknowledgements

The subject of this work starts from the ideas of my thesis advisors, Dr. Josep Costa Balanzat and Pedro Manuel Ponces Rodrigues de Castro Camanho. Their excellent ideas, advice and support were invaluable for the completion of this work and I render thanks to them.

I would like to express my gratitude to Carlos D´avila for his continuous interest in the work and his valuable comments and contributions that were very constructive.

I would also like to thank him for having offered me the possibility to visit NASA Langley during the summers of 2004 and 2005.

A la Universitat de Girona he tingut la possibilitat de treballar en el grup de recerca AMADE, on en tot moment m’han facilitat la feina. Voldria agra¨ır a en Narc´ıs Gascons, que fou qui em va introduir dins AMADE. Agra¨ır especialment l’amistat, els consells i la seva sempre bona disposici´o d’en Joan Andreu, en Jordi Renart, en Pere Maim´ı, en Pep, en Benigne, en Norbert, en Dani, l’Elio, en Sergi, l’Emili, la Montse i la Marta, tots plegats hem passat bones estones.

I would also like to thank you Cassilda and Sukdee with whom I have shared the different phases of the research stages in Porto and in Hampton, respectively.

Voldria agra¨ır tamb´e el suport dels meus amics, en Santi, en Sergi, la Maria, la Gemma, la Yolanda, en Toni, la Carme i especialment a en Dani pel seu continu inter´es. De les dues preguntes que sempre em feieu: de qu`e va la tesi? quan acabar`as?

ara si que ja puc respondre la segona. Per la primera us deixo que la llegiu!

Un agra¨ıment profund als meus pares, Lloren¸c i Isabel, la meva `avia Francesca i especialment a la meva germana Margarita pels inestimables `anims i el seu continu suport.

Finalment, el meu m´es sincer agra¨ıment a l’Anna. Ella va ser qui m´es em va esperonar a emprendre aquest viatge i la seva paci`encia, comprensi´o i recolzament m’han ajudat molt durant tot aquest temps.

## Contents

List of Figures 5

List of Tables 11

1 Introduction and objectives 15

### I Delamination under quasi-static loading 21

2 Delamination in composite materials 23

2.1 Introduction . . . 23

2.1.1 Origin of delamination . . . 23

2.1.2 Types of delamination . . . 24

2.2 Micromechanics of delamination . . . 26

2.3 Approaches to delamination . . . 28

2.3.1 Fracture Mechanics approach . . . 29

2.3.2 Cohesive or Damage Zone Models . . . 31

3 Interface damage model 39 3.1 Introduction . . . 39

3.2 Model for delamination onset and propagation . . . 41

3.2.1 Boundary value problem . . . 41

3.2.2 Kinematics of the interfacial surface . . . 42

3.2.3 Constitutive laws . . . 44 1

3.2.4 Formulation of the constitutive tangent tensor . . . 55

3.3 Finite element discretization - computational model . . . 56

3.3.1 Discretization of the interfacial surface . . . 57

3.4 Comparison with experimental studies . . . 59

3.4.1 Mode I, mode II and mixed-mode I and II delamination . . . . 60

3.4.2 Skin-stiffener co-cured structure . . . 66

3.5 Concluding remarks . . . 70

4 Analysis of the mesh size influence 71 4.1 Introduction . . . 71

4.2 Selection of cohesive zone model parameters . . . 72

4.2.1 Cohesive zone model and FEM . . . 72

4.2.2 Guidelines for the selection of the parameters of the interface with coarser meshes . . . 78

4.3 Simulation of the double cantilever beam specimen . . . 80

4.3.1 Effect of interface strength . . . 84

4.3.2 Effect of interface stiffness . . . 86

4.4 Simulation of free-edge delamination . . . 87

4.4.1 Problem statement . . . 87

4.4.2 Numerical predictions . . . 89

4.5 Concluding remarks . . . 93

### II Delamination under fatigue loading 95

5 Fatigue in composite materials 97 5.1 Fatigue modeling . . . 975.1.1 Fatigue life models . . . 98

5.1.2 Fracture Mechanics models . . . 99

5.1.3 Damage Mechanics models . . . 101

5.2 Fatigue delamination of composite laminates . . . 104

5.2.1 Introduction . . . 104

5.2.2 Fatigue growth of interlaminar cracks . . . 104

5.2.3 Simulation of fatigue delamination of composite laminates . . 109

6 Simulation of fatigue delamination 117 6.1 Introduction and motivation . . . 117

6.2 Cohesive Zone Model approach . . . 118

6.2.1 Numerical implementation of to the CZM . . . 119

6.3 Constitutive model for high-cycle fatigue . . . 120

6.3.1 Determination of the growth rate of the damaged area as a function of the number of cycles . . . 121

6.3.2 Evolution of the damage variable under cyclic loading . . . 123

6.3.3 Crack growth rate . . . 123

6.3.4 Cycle jump strategy . . . 126

6.4 Results and discussion . . . 127

6.4.1 One element tests . . . 128

6.4.2 Simulation of a DCB specimen under fatigue loading . . . 130

6.4.3 Simulation of a 4ENF test . . . 135

6.4.4 Simulation of mixed-mode loading . . . 139

6.5 Conclusions . . . 142

### III Closure 143

7 Conclusions and Future Work 145 7.1 Conclusions . . . 1457.1.1 Cohesive zone model for the simulation of delamination under quasi-static loads . . . 145

7.1.2 Cohesive zone model for the simulation of delamination under

high-cycle fatigue . . . 147

7.2 Suggestions for Future Work . . . 148

7.2.1 Quasi-static Model . . . 148

7.2.2 Fatigue Model . . . 148

7.2.3 Environmental Effects . . . 149

7.2.4 Stochastic Distributions . . . 150

### IV Appendices 151

A Cohesive element User Manual 153 A.1 Preface . . . 154A.2 Introduction . . . 154

A.3 Formulation of the Element . . . 154

A.3.1 Basic element theory . . . 154

A.3.2 Element definition . . . 156

A.3.3 Implementation status . . . 157

A.4 Input into ABAQUS/Standard . . . 159

A.4.1 Element type . . . 159

A.4.2 Number of nodes and coordinates per node . . . 159

A.4.3 Element properties . . . 159

A.4.4 Number of solution-dependent variables . . . 161

A.5 Examples . . . 161

A.5.1 One element simulations . . . 162

A.5.2 Mode I, mode II and mixed-mode delamination growth for PEEK composites . . . 164

B Code 167

C Input files 181

C.1 One element simulations . . . 181

C.1.1 Input file for an 8-node decohesion element that connects two three dimensional continuum elements. . . 181

C.1.2 Input file for an 4-node decohesion element that connects two continuum plane strain element . . . 184

C.1.3 Input file for an 4-node decohesion element that connects two
continuum plane strain element. Rotated 90^{o}. . . 186

C.2 Mode I, mode II and mixed-mode delamination . . . 188

C.2.1 Input file for the DCB test. . . 188

C.2.2 Input file for the ENF test. . . 191

C.2.3 Input file for the MMB 80 test. . . 194

Bibliography 198

## List of Figures

*1.1 Building block integration of the certification methodology (Mil-Hbk-17*
*[1]) and reduction on the test requeriments through Virtual Mechani-*
*cal Testing. . . 16*

*2.1 Internal delamination: (a) disposition across the laminate and (b)*
*effect on the overall stability (Figure from Bolotin [6]). . . 25*

*2.2 Near-surface delamination: (a) open in tension; (b) closed in tension;*

*(c) open buckled; (d) closed buckled; (e) edge buckled and (f) edge*
*buckled with secondary crack (Figure from Bolotin [6]). . . 26*

*2.3 Mode I, mode II, and mode III crack propagation modes. . . 27*
*2.4 Formation and growth of a mode II delamination at the ply inter-*

*face: (a) microcrack formation ahead of the crack tip; (b) microcrack*
*growth and opening and (c) microcrack coalescence accompanied by*
*shear cusps [9]. . . 28*

*2.5 Calculation of the energy release rate using Virtual Crack Closure*
*Technique. . . 30*

*2.6 Tractions in the cohesive zone ahead of the crack tip. . . 32*
*2.7 Equivalence between the physical cohesive model and the numerical*

*cohesive model. . . 35*

7

*2.8 Traction-relative displacement curves employed in various models in*

*the literature (Figure from Zou et al.[66]). . . 37*

*3.1 Restoration of the cohesive state for delamination propagation under*
*variable mode-ratio. . . 40*

3.2 *Body Ω crossed by a material discontinuity Γ*_{d}*in the undeformed*
*configuration. . . 41*

*3.3 Interfacial surface deformation. . . 43*

*3.4 Energy dissipation during damage evolution. . . 46*

*3.5 A bilinear constitutive equation for the cohesive element for a mixed-*
*mode loading situation. . . 49*

*3.6 Comparison between Ye’s criterion, a maximum traction criterion*
*and the new proposed criterion. . . 53*

*3.7 Isodamage curves in the relative displacements space. . . 54*

*3.8 MMB test specimen. . . 60*

*3.9 Numerical and experimental results- pure mode I loading. . . 63*

*3.10 Numerical and experimental results- mixed-mode I and II loading with*
*G**II**/G**T**=20%. . . 63*

*3.11 Numerical and experimental results- mixed-mode I and II loading with*
*G*_{II}*/G*_{T}*=50%. . . 64*

*3.12 Numerical and experimental results- mixed-mode I and II loading with*
*G*_{II}*/G*_{T}*=80%. . . 64*

*3.13 Numerical and experimental results- pure mode II loading. . . 65*

*3.14 Skin-stiffener test specimen. . . 66*

*3.15 Skin-Stiffener debonding. . . 68*

*3.16 Experimental and numerical load-extensometer displacement relations. 69*

*4.1 Influence of the cohesive surface on the deformation. . . 73*
*4.2 Distribution of tractions ahead of the crack tip at peak load. . . 81*
*4.3 Load-displacement curves using the nominal interface strength (τ*^{0}*=60MPa)*
*for a DCB test with different mesh sizes. . . 83*

*4.4 Distribution of tractions ahead of the crack tip for an applied load of*
*30kN. . . 84*
*4.5 Load-displacement curves obtained for a DCB test with different mesh*

*sizes with the interface strength modified to keep N*_{e}*≥5. . . 85*
*4.6 Maximum load obtained in a DCB test for two cases: a) with constant*

*interfacial strength, b) with interfacial strength calculated according*
*to Eq. (4.9). . . 86*
*4.7 Influence of the interface stiffness on the load-displacement curves. . . 87*
*4.8 Cross-section of the laminate. . . 88*
*4.9 Load-displacement curves obtained for a free-edge test with different*

*mesh sizes using nominal interface strength properties. . . 90*

*4.10 Evolution of stresses during delamination onset and propagation of*
*the two interior layers of the laminate. . . 90*

*4.11 Load-displacement curves obtained for a free-edge test with different*
*mesh sizes and with the interface strength adjusted for N*_{e}*=5. . . 92*
*4.12 Load-displacement curves obtained for a free-edge test with different*

*mesh sizes and with the interface strength adjusted for N*_{e}*=10. . . 92*
*4.13 Maximum load obtained in a free-edge test for three cases: a) with*

*constant interfacial strength, b) and c) with interfacial strength cal-*
*culated according to Eq.(4.9) with N*_{e}*equal to 5 and 10. . . 93*

*5.1 Typical crack growth rate pattern.* . . . 101

*5.2 Delamination onset surface for IM7/8552 mixed-mode I/II fatigue*
*failure [154]. . . 110*

*6.1 Linear softening law for a cohesive zone model approach. . . 119*
*6.2 Equivalence between the physical (left) and numerical (right) consti-*

*tutive equation of the CZM. . . 120*

*6.3 Schematic representation of the equivalence between the increase in*
*the damaged area and the crack growth.* . . . 122
*6.4 Variation of the energy release rate.* . . . 125
*6.5 The load ratio effect is captured by the constitutive equations. The*

*higher load ratios (R*_{1} *> R*_{2}*) the smaller ∆G (∆G*_{2} *> ∆G*_{1}*). . . 126*
*6.6 Undeformed mesh with the boundary conditions and deformed mesh*

*of one cohesive element tests. . . 128*

*6.7 Evolution of the interface traction in the constitutive equation for a*
*displacement jump controlled high-cycle fatigue test.* . . . 129
*6.8 Evolution of the interface traction and the maximum interface strength*

*as a function of the number of cycles for a displacement jump con-*
*trolled high-cycle fatigue test. . . 130*

*6.9 Loading pattern for Mode I specimen.* . . . 131
*6.10 Detail of the FEM model of the DCB specimen. Two applied load P*

*with opposite direction were applied to each arm. The applied moment*
*is equal to the product between the applied load P and the thickness*
*of the arm. . . 132*

*6.11 Comparison of the experimental data with the crack growth rate ob-*
*tained from the numerical simulation for a Mode I DCB test.* . . . . 134

*6.12 Sensitivity of the model to the load ratio for a Mode I DCB test.* . . 135
*6.13 Sensitivity of the model to the load ratio for a Mode I DCB test.* . . 136
*6.14 Loading pattern for Mode II 4ENF specimen.* . . . 136
*6.15 Detail of the FEM model of the 4ENF specimen.* . . . 137
*6.16 Comparison of the experimental data with the crack growth rate ob-*

*tained from the numerical simulation for a Mode II 4ENF test.* . . . 138
*6.17 Loading pattern for mixed-mode specimen. . . 139*
*6.18 Detail of the FEM model of the specimen mixed-mode loaded.* . . . . 140
*6.19 Comparison of the experimental data with the crack growth rate ob-*

*tained from the numerical simulation for a mixed-mode test with G** _{I}* =

*G*

*II*

*. . . 141*

A.1 Element node-numbering conventions . . . 156
*A.2 A bilinear constitutive equation for the cohesive element for a mixed-*

*mode loading situation . . . 158*
A.3 Undeformed and deformed mesh of models with an 8-node cohesive

element (left), and a 4-node cohesive element (center and right), con- necting two continuum elements. . . 162 A.4 Load-displacement curve for models with one cohesive element . . . . 163 A.5 Undeformed and deformed mesh for the MMB simulation . . . 165 A.6 Load-displacement curves for DCB, ENF and MMB 80% tests . . . . 165

## List of Tables

*3.1 Ply properties. . . 61*
*3.2 Experimental data. . . 61*
*3.3 Maximum loads. . . 65*
*3.4 Material properties for IM6-3501-6 unidirectional graphite epoxy.* . . 67
*3.5 Interface properties for IM6-3501-6 unidirectional graphite epoxy. . . 67*
*3.6 Comparison between experimental and numerical results. . . 68*
*4.1 Interface stiffness K proposed by different authors (N/mm*^{3}*) and those*

*calculated from Equation (4.4). . . 75*
*4.2 Length of the cohesive zone and equivalent value of the parameter M.* 77
*4.3 Mechanical and interface material properties of T300/977-2 [48],[110]. 81*
*4.4 Mechanical properties of T300/934 Graphite Epoxy [111], [114]. . . . 88*
*4.5 Summary of predicted and experimental values of tension tests on*

*T300/934 laminates. . . 91*

*6.1 Properties used in the models with only one cohesive element.* . . . . 128
*6.2 Material properties for HTA/6376C carbon/epoxy [140, 167, 168].* . 131
*6.3 Fatigue material properties for HTA/6376C carbon/epoxy obtained*

*from references [140, 168] and using Equations (6.20) to (6.22).* . . 133

13

## Chapter 1

## Introduction and objectives

The structural applications of polymer-matrix composite materials reinforced with continuous fibres are gradually expanding as a result of the mechanical properties of these materials (e.g. excellent stiffness/weight and strength/weight ratios, easy formability, and corrosion resistance). Aerospace and aeronautics can be considered to be the pioneering industries in the application of this type of composites, although nowadays composite materials are used as base materials in the most advanced products of many sectors such as naval engineering, civil engineering, automobile industry, sporting equipment, etc.

The application of composites in structural components (e.g. main load-bearing structures of aircraft) is still limited by the difficulty in predicting their service lives.

In fact, whilst military aircrafts are mainly built with composite materials, civil aircrafts still use metals in several structural components. As the understanding of its behaviour improves, the use of composite materials spreads. However, the usual methodology for the determination of their reliability, which implies a large number of tests in real-size structural components, is only suitable in sectors with a large added value, such as aeronautics, that can afford the design and certification costs. Moreover, existing mechanical tests are not always able to reproduce all the possible circumstances that will be encountered during service life (environmental conditions, cyclic loads, load combination, etc.). To increase the reliability and to

15

decrease the the number of required tests to certify a composite structure (see Figure 1.1), efficient design tools are needed. These tools must be robust, efficient, and carefully validated against test data to ensure that they are capable of predicting consistently the response of components in service. Such capability to substitute some of the mechanical test with accurate computer simulations is referred to as

“virtual mechanical testing”. The development of this kind of tools needs a deep knowledge of the material behaviour.

*Figure 1.1: Building block integration of the certification methodology (Mil-Hbk-17*
*[1]) and reduction on the test requeriments through Virtual Mechanical Testing.*

Moreover, the philosophy behind the design of advanced components differs from the conventional methodology to design structural components. While the conven- tional approach is based on a strength verification, i.e, the ability of the structure or the material to resist the damage occurrence; the new concepts are also based on a damage-tolerance verification besides the strength verification, i.e. the damaged material should maintain the functionality after damage occurrence. The damage- tolerance approach allows for the presence of subcritical cracks that will not grow to critical length between periodic inspections. The damage-tolerance concept pro- vides quantitative guidance for balancing of the cost of repair or replacement of a damaged component against the possibility that continued service could lead to failure.

The strength-based design relies on the obtention of “design allowable values”, generally obtained from a selected experimental tests and corrected by safety factors (or uncertainty factors). These uncertainty factors are used to consider the varia- tions between the constraints considered in the design (variations in the material properties, environmental effects, load combination, etc.) and the real conditions of the component or structure in service. Usually, the design allowable values are obtained for static loading while fatigue loading is taken into account in the design through the increase of the safety factor.

However, the damage-tolerance approach requires the use of techniques that al- low to predict both crack initiation and growth to verify that subcritical cracks will not grow to critical lengths between periodic inspections. In-service loads of the real components or structures are mostly of cyclic origin. Under these circumstances, damage-tolerance approach is especially important in real structures loaded under fatigue conditions, where the growth of subcritical cracks is the main cause of fail- ure. The experimental characterization of the fatigue behavior of large components requires a large number of tests. Therefore, the development of complete and effi- cient design tools that take into account fatigue loading can significantly reduce the development costs. Moreover, damage-tolerance techniques allow to schedule the

maintenance or replacement of components before catastrophic failure.

The design of primary and secondary composite structures for aeronautical ap- plications involves both concepts, strength and damage-tolerance. The development of specific tools for composites that are able to predict the strength and damage- tolerance is still a problem under investigation.

The special microstructural characteristics of composites (anisotropy, hetero- geneity, the existence of a matrix/fibre interface with its own properties and the presence of defects) creates difficulties in the development of constitutive models to assist structural design.

The usual failure mechanisms in composites can be divided in: i) fibre failure modes, tensile fracture or local compressive kinking; ii) matrix failure modes, gener- ally matrix cracking although other effects such as degradation caused by radiation or by moisture uptake should be taken into account; iii) fibre/matrix interface failure or fibre/matrix debonding; iv) inter-laminar interface failure, or cracks caused by the loss of adhesion between two consecutive laminae, normally called delamination.

Among these different failure mechanisms, delamination is one of the most common types of damage in laminated fibre-reinforced composites due to their relatively weak interlaminar strengths. Delamination may arise under various circumstances, such as in the case of transverse concentrated loads caused by low velocity impacts.

This damage mode is particularly important for the structural integrity of composite structures because it is difficult to detect during inspection. Furthermore, delamina- tion causes a drastic reduction of the bending stiffness of a composite structure and, when compressive loads are present, promotes local buckling that can compromise the global stability of the structure.

The initiation of a delamination-like defect does not necessarily mean that a structural component is at, or even near, the end of its useful service life. An efficient design tool able to predict the initiation of a delamination could improve the design based on strength criteria. On the other hand, models of interlaminar crack growth improve the design oriented to damage-tolerance and provide decision

tools for the definition of the repair/subsitution of damaged structures [2].

Reliable and efficient design tools are needed to improve the design and decrease the development cost of a composite component. These tools need to be developed using the damage-tolerance approach to take into account all of the stages of the composite component during its lifetime. The design tools must take into account fatigue loading, which is the most typical nature of the in-service loads. The de- velopment of accurate and general design tools requires the study of delamination under static and fatigue loading. To facilitate the widespread use of advanced design tools, they have to be implemented in numerical methods normally used in the de- sign of structures (such the Finite Element Method) and accessible to the majority of the designers.

The objective of this thesis is to develop an effective design tool to analyze delamination onset and growth in advanced composite materials under quasi–static and fatigue loading.

The methodology used to pursue this objective is structured as follows. The thesis is divided in two parts: the numerical tools to simulate delamination under quasi-static loading are described in Part I; the numerical tools to simulate delami- nation under fatigue loading are described in Part II.

Part I comprises Chapters 2 through 4, and it is structured as follows. Chap- ter 2 describes the phenomena of delamination under quasi-static loading and the different approaches used in the literature to deal with the problem. This informa- tion is essential to define the approach adopted: a finite element formulation of a cohesive element by means of the Cohesive Zone Model (CZM) approach. The liter- ature reports a considerable number of approaches to the simulation of delamination under static or quasi-static loading. Several cohesive zone formulations present an inconsistency when the mode-ratio changes. Moreover, the application of the mod- els present in the literature involve important mesh requirements to obtain accurate results. These mesh requirements are computationally heavy and can make the simulation of full-size components or structures intractable.

A thermodynamically consistent cohesive damage model that accounts for vari- ations in the mode-ratio is presented in Chapter 3. The finite element discretization of the boundary value problem is also described. The model is validated with exper- imental data of standard tests and used to simulate the response of a skin-stringer configuration frequently used in aircraft structures.

Chapter 4 proposes a methodology to decrease the mesh size requirements in cohesive zone models. The chapter presents a methodology to use CZM in the simulation of delamination in large structures used in the industry where the re- quirements of extremely fine meshes cannot be met. By adjusting the parameters of the cohesive zone model, it is shown that it is possible to predict delamination ac- curately in specimens with and without pre-existing cracks by using coarser meshes than usual.

Part II comprises Chapters 5 and 6, and it is structured as follows. Chapter 5 first reviews the different approaches used to study the phenomena of fatigue.

Then, the effect of fatigue delamination in composite materials is described and the different approaches present in the literature presented. This information is the basis for the definition of the approach adopted: a high-cycle fatigue model to simulate delamination under cyclic loading.

Chapter 6 describes the high-cycle fatigue model developed. The model is vali- dated with experimental data, and the sensitivity of the model to load-dependent parameters like the stress ratio or the mode-ratio is analyzed.

The thesis is concluded in Chapter 7 with an overall assessment of its achieve- ments and a discussion of possible avenues for future developments.

The models developed are implemented as a user-written element in the com-
mercial finite element code ABAQUS^{°}^{c}. The details of the code, some examples of
input files and a User Manual are given in the Appendices.

## Part I

## Delamination under quasi-static loading

21

## Chapter 2

## Delamination in composite materials

### 2.1 Introduction

Delamination is one of the most common types of damage in laminated fibre- reinforced composites due to their relatively weak interlaminar strengths. Delam- ination can form during any moment of the life of the structure: manufacturing, transport, mounting and service.

### 2.1.1 Origin of delamination

According to Pagano and Schoeppner [3] the technological causes of the delamination can be grouped in two categories. The first category includes delamination due to curved sections, such as curved segments, tubular sections, cylinders and spheres, and pressurized containers. In all of these cases, the normal and shear stresses at the interface of two adjacent plies can originate the loss of adhesion and the initiation of an interlaminar crack.

The second category includes abrupt changes of section, such as ply drop-offs, unions between stiffeners and thin plates, free edges, and bonded and bolted joints.

23

A third category related to temperature and moisture effects can be added. The difference between the thermal coefficients of matrix and reinforcement results in differential contractions between the plies during the curing process of the laminate.

The residual stresses originated by these differential contractions might be a source of delamination [4]. Similarly, the different expansion of the plies of the laminate during the absorption of moisture might be a cause for delamination [5].

Delamination may also originate during the manufacturing stage due to the shrinkage of the matrix during curing, or due to the formation of resin-rich areas that result from poor practices when laying the plies. [6, 7].

During service, delamination may arise under various circumstances, such as in the case of transverse concentrated loads caused by low velocity impacts. Impact is an important source of delamination in composite structures. Interlaminar cracks can originate from internal damage in the interface between adjacent plies as a consequence of impact, from the drop of a tool during production, mounting or repairing, or from ballistic impacts in military planes or structures.

### 2.1.2 Types of delamination

According to Bolotin [6, 7], two types of delamination can be considered: internal delaminations and near-surface delamination. Internal delamination originate in the inner ply interfaces of the laminate and can be due to the interaction of matrix cracks and ply interfaces. Delaminations originated by transverse matrix cracks in plies orthogonal to the tensile load are common examples of this type of delamination.

Internal delamination reduces considerably the load-capacity of composite struc- tures. In particular, when compression loads are applied, the overall flexural be- haviour of the laminate is significantly affected (as shown schematically in Figure 2.1). Although delamination separates the laminate in two parts, there is an inter- action between the deformation of the one part of the laminate and the other. Due to this interaction, both parts of the laminate may deflect in a similar way.

*Figure 2.1: Internal delamination: (a) disposition across the laminate and (b) effect*
*on the overall stability (Figure from Bolotin [6]).*

Near-surface delaminations, as the name indicates, originate near the surface of the laminate and represent a more complex scenario than internal delaminations.

The deformation of the delaminated part is less influenced by the deformation of the rest of the laminate. Therefore, the deformation of the near-surface delaminated part does not necessary follow the deformation of the rest of the laminate. Consequently, not only the growth of the near-surface delamination has to be taken into account but also its local stability. Bolotin [6, 7] classified the different types of near-surface delamination than can originate in plate composite components in different load conditions as shown in Figure 2.2.

After initiation, internal o r near-surface delaminations can propagate under either static or fatigue loads. In both cases, the reduction in strength and stability of the composite part to flexural loading is considerable. In addition, the delamination damage mode is particularly important for the structural integrity of composite structures because it is difficult to detect during inspection.

*Figure 2.2: Near-surface delamination: (a) open in tension; (b) closed in tension;*

*(c) open buckled; (d) closed buckled; (e) edge buckled and (f) edge buckled with*
*secondary crack (Figure from Bolotin [6]).*

### 2.2 Micromechanics of delamination

At the microscopic level, the growth of an interlaminar crack is preceded by the formation of a damage zone ahead of the crack tip. The size and shape at the deformation/damage zone is seen to be quite variable, depending on both the resin toughness and the state of stress (mode I, mode II, mode III or mixed-mode, see Figure 2.3). The damage zone ahead of the crack tip for mode II or mode III loading is greater than for mode I loading. A much slower decaying of the stress field ahead of the crack tip for the shear modes of loading is responsible for this difference. On the other hand, there are differences between systems with brittle or ductile matrices: the deformation/damaged zone for more brittle composites is much smaller.

For mode I loading in brittle systems, the zone ahead of the crack tip contains microcracks whose coalescence and growth results in crack advance. Sometimes,

crack advance occurs by fibre-matrix debonding before microcrack coalescence oc- curs. When debonding takes place, fibre bridging and fiber breakage are observed.

For ductile systems, plastic deformation around the crack tip precedes crack ad- vance. Crack advanc generally occurs by ductile tearing, but crack advance by interfacial debonding was also commonly observed in composites made with more ductile resins [8].

Mode I Mode II Mode III

*Figure 2.3: Mode I, mode II, and mode III crack propagation modes.*

Shear mode delamination (mode II and/or mode III) of quasi-brittle systems
occurs in a very distinctive way. Microcracks form from a considerable distance
ahead of the crack tip, at a 45^{o}-angle to the plane of the ply. These cracks grow until
they reach the fibres, which bound the resin-rich region between plies. It sometimes
appears that the cracks stop in the resin short of the nearest visible fiber. However
there are certainly fibers just at the top or beneath the surface that are responsible
for arresting these growing microcracks. Coalescence of these microcracks is required
for macrocrack advance. This coalesce generally occurs at the fiber/matrix interface,
giving a “corrugated roof appearance” along with the formation of “hackles” in the
resin between fibers (see Figure 2.4). The fracture process for mode II delamination
appears to be ductile rupture, with occasional fibre debonding.

*Figure 2.4: Formation and growth of a mode II delamination at the ply interface:*

*(a) microcrack formation ahead of the crack tip; (b) microcrack growth and opening*
*and (c) microcrack coalescence accompanied by shear cusps [9].*

### 2.3 Approaches to delamination

Historically, the delamination mechanics was first studied by Obreimoff (1894-1981), a Soviet expert in the field of solid-state physics. In 1930, he published in an English journal a paper under the title “The Splitting Strength of Mica” [10]. Obreimoff estimated the specific work of interlaminar fracture, examining the detaching of a layer from a mica specimen under the action of a tearing force. The paper followed the series of pioneering papers by Griffith in 1920. From the early 1980’s and up to the present day, the delamination mechanics has been a subject of ever-increasing interest. The number of studies in this field runs into thousands.

The procedures used for the numerical simulation of the delamination can be divided into two groups. The first group is based on the direct application of Frac- ture Mechanics, while the second formulates the problem within the framework of Damage Mechanics.

### 2.3.1 Fracture Mechanics approach

When other material non-linearities can be neglected, methods based on Linear Elastic Fracture Mechanics (LEFM) have been proven to be effective in predicting delamination growth. However, LEFM cannot be applied without an initial crack.

In some situations, methods combining a stress analysis with a characteristic dis- tance have been applied to predict the initiation of delamination [11, 12]. After delamination onset, LEFM can be used to predict delamination growth [13, 14].

Techniques such as the Virtual Crack Closure Technique (VCCT) [15]–[19], the J- integral method [20], the virtual crack extension [21] and stiffness derivative [22]

have often been used to predict delamination growth. These techniques are used to calculate the components of the energy release rate. Delamination growth is pre- dicted when a combination of the components of the energy release rate is equal to, or greater than, a critical value [23]. However, difficulties are also encountered when these techniques are implemented using finite element codes. The calculation of fracture parameters, e.g. stress intensity factors or energy release rates, requires nodal variable and topological information from the nodes ahead and behind the crack front. Such calculations can be done with some effort for a stationary crack, but can be extremely difficult when progressive crack propagation is involved.

Virtual Crack Closure Technique (VCCT)

The virtual crack closure technique is one of the most widely used procedures to
predict crack propagation. This technique is based on Irwin’s assumption that when
a crack extends by a small amount, the energy released in the process is equal to the
work required to close the crack to its original length. If the energy released per unit
*area is greater than or equal to the critical value, G** _{c}*, the crack will propagate. The

*mode I, mode II and mode III energy release rates, G*

_{I}

*, G*

_{II}

*and G*

_{III}, respectively, can be computed from the nodal forces and displacements obtained from the solution of a finite element model [18, 19].

In a finite element model such as shown in Figure 2.5, the energy released is the work done by the nodal forces required to close the crack tip, therefore:

*G*_{I} = 1

*2b∆aF*_{cd}^{y}*(v*_{c}*− v** _{d}*) (2.1)

*G*

_{II}= 1

*2b∆aF*_{cd}^{x}*(u*_{c}*− u** _{d}*) (2.2)

*G*

_{III}= 1

*2b∆aF*_{cd}^{z}*(w*_{c}*− w** _{d}*) (2.3)

*where b is the specimen thickness, F*_{cd}^{y}*, F*_{cd}^{x}*, and F*_{cd}* ^{z}* are the magnitudes of nodal

*forces pairs at nodes c and d in the y,x and z direction, respecitvely. u*

_{c}*, v*

_{c}*, w*

*and*

_{c}*u*

_{d}*.v*

_{d}*, w*

_{d}*are the nodal displacements before nodes c and d are pulled together.*

*Figure 2.5: Calculation of the energy release rate using Virtual Crack Closure Tech-*
*nique.*

The analysis can be done in two steps, using the first step to compute the values
*of the nodal forces F*_{cd}^{y}*, F*_{cd}^{x}*and F*_{cd}^{z}*necessary to hold the nodes c and d together,*
*while the relative displacement components between nodes c and d are computed in*
the second step. However the analysis can be simplified using the assumption made
by Rybicki and Kanninen [16], who suggested that the values of the nodal forces in
equations (2.1), (2.2), and (2.3) can be replaced by the corresponding components
*of nodal forces F*_{ef}^{y}*, F*_{ef}^{x}*and F*_{ef}* ^{z}* .

*After the calculation of G*_{I}*, G*_{II} *and G*_{III}, the total energy release rate reads:

*G*_{T}*= G*_{I}*+ G*_{II}*+ G*_{III} (2.4)

Crack propagation is predicted when the computed energy release rate is equal
*to the fracture toughness of the material, G** _{c}*:

*G*_{T}*= G** _{c}* (2.5)

One advantages of this form of calculation is that it is based on energy rather
than stress. The main drawback of the VCCT technique is that it is based on the
*assumption of self-similar propagation, i.e. the forces F*_{ef}^{i}*and F*_{cd}* ^{i}* are the same.

Therefore, crack initiation and the propagation of short cracks cannot be predicted.

only crack propagation could be predicted, regardless of crack initiation.

### 2.3.2 Cohesive or Damage Zone Models

Another approach for the numerical simulation of delamination can be developed within the framework of Damage Mechanics. Models formulated using Damage Mechanics are based on the concept of the cohesive crack model: a cohesive damage zone is developed near the crack front. The origin of the cohesive crack model goes back to Dugdale [24] who introduced the concept that stresses in the material are limited by the yield stress and that a thin plastic zone is generated in front of the notch. Barenblatt [25] introduced cohesive forces on a molecular scale in order to solve the problem of equilibrium in elastic bodies with cracks. Hillerborg et al. [26]

proposed a model similar to Barenblatt’s model, but where the concept of tensile strength was introduced. Hillerborg’s model allowed for existing cracks to grow and, more importantly, also allowed for the initiation of new cracks.

Cohesive damage zone models relate tractions to displacement jumps at an in-
terface where a crack may occur (see Figure 2.6). Damage initiation is related to the
*interfacial strength, i.e., the maximum traction τ*^{o} in the traction-displacement jump

relation. When the area under the traction-displacement jump relation is equal to
*the fracture toughness G** _{c}*, the traction is reduced to zero and new crack surfaces
are formed.

*Figure 2.6: Tractions in the cohesive zone ahead of the crack tip.*

The advantages of cohesive zone models are its simplicity and the unification of crack initiation and growth within one model. Although the cohesive damage models cannot be considered non-local damage models [27], they allow a mesh-independent representation of material softening, provided that the mesh is sufficiently refined.

These aspects are discussed in more detail in Chapter 4.

Cohesive Zone Model formulations are more powerful than Fracture Mechanics approaches because they allow the prediction of both initiation and crack propaga- tion, and thus, damage tolerance and strength analyses can be done with the same design tool.

Pure mode loading

Under pure mode I, mode II, or mode III loading, delamination initiation occurs
when the corresponding interlaminar traction is equal to its respective maximum
*interfacial strength (τ*_{3}^{o}*, τ*_{2}^{o}*, τ*_{1}* ^{o}*)

*τ*_{i}*= τ*_{i}^{o} (2.6)

*Delamination propagation is predicted when the energy release rate (G*_{I}*, G*_{II}
*or G*_{III}*) is equal the corresponding fracture toughness of the material (G*_{Ic}*, G*_{IIc} or
*G*_{IIIc}). Thus, equations (2.6) and (2.5) define the initiation and propagation criteria,
respectively. The transition between the delamination initiation and delamination
propagation is controlled by the constitutive equation.

Mixed-mode loading

For mixed-mode loading, the coupling effects between loading modes must be taken into account. For an undamaged interface, delamination starts when a scalar func- tion of the interlaminar stresses reaches a limit. The conventional stress-based failure criterion is only suitable for predicting damage initiation:

f*initiation* *= f (τ**i**) − 1 = 0* (2.7)

where f_{initiation}*is the failure criterion and f (τ** _{i}*) is a norm of the tractions. Few
models take into account the interaction of the traction components in the predic-
tion of damage onset. The models that account for the interaction of the traction
components are usually based on Ye’s criterion [28], using a quadratic interaction
of the tractions:

f* _{initiation}*=
µ

*hτ*3

*i*

*τ*_{3}^{o}

¶_{2}
+

µ*τ*2

*τ*_{2}^{o}

¶_{2}
+

µ*τ*1

*τ*_{1}^{o}

¶_{2}

*− 1 = 0* (2.8)

*where h·i is the MacAuley bracket defined as hxi =* ^{1}_{2}*(x + |x|).*

The criterion for propagation is often formulated independently of the criterion for initiation. The failure criterion for delamination propagation can be expressed as:

f*propagation**= f (G*_{i}*) − 1 = 0* (2.9)

where f*propagation**is a function of the pure mode fracture energies and f (G** _{i}*) is a norm
of the energy release rates. There are different forms adopted in the literature to
define the propagation criteria. One of these criteria is the power law expression:

f*propagation**(G**i*) =
µ*G*_{I}

*G*_{I}

¶* _{α}*
+

µ*G*_{II}
*G*_{II}

¶* _{β}*
+

µ*G*_{III}
*G*_{III}

¶_{γ}

*− 1 = 0* (2.10)

*where G*_{I}*, G*_{II} *or G*_{III} *are the individual components of energy release rate, and α, β,*
*and γ are parameters to be fit with experimental data. The values α = β = γ = 1 or*
*α = β = γ = 2 are frequently chosen when no experimental data is available. The*
*values α = β = γ = 1 correspond to a linear failure criterion, and α = β = γ = 2*
correspond to a quadratic failure criterion.

Kenane and Benzeggagh [29] proposed a failure criterion which, in some cases, fits experimental results more accurately:

f*propagation* = *G*_{T}

*G*_{c}*− 1 = 0* (2.11)

*where G*_{T}*is obtained with Equation (2.4) and G** _{c}* is

*G*_{c}*= G*_{Ic}*+ (G*_{IIc}*− G*_{Ic})

µ*G*_{I}*+ G*_{I}
*G*_{T}

¶_{η}

(2.12)

*where η is a parameter found by fitting Equation (2.12) to the experimental data.*

Kim [30] proposes a modification of Equation (2.13):

*G**c**= 2G*Ic*+ (G*IIc*− G*Ic)

µ*G*_{I}*+ G*_{I}
*G*_{T}

¶_{η}

(2.13)

Numerical implementation of Cohesive Zone Model

Cohesive Zone formulations are well-suited to be implemented in finite element codes. However, the traction-displacement jump relation presented in Figure 2.6

has to be modified to be implemented in a Finite Element code by means of stan- dard interface elements. An elastic path is introduced in the constitutive equation as shown in Figure 2.7 before damage initiation. This linear elastic part introduces a very high stiffness to the interface before damage initiation.

*Figure 2.7: Equivalence between the physical cohesive model and the numerical co-*
*hesive model.*

There are two main strategies in the literature to implement cohesive zone for- mulations: discrete interelement cracks and discrete intralement cracks.

In the first strategy, the crack extends between elements and remeshing is nec- essary when the crack path is not known in advance. This approach has been used to model cohesive crack growth in concrete [31]-[33] and to model crack growth in ductile materials [34, 35]. Xu et al. [36] and Camacho et al. [37] placed the cohesive zone as an interelement in between each pair of neighboring elements in the mesh.

This idea is widely used in the simulation of delamination in multilayered materials using interface or so-called cohesive elements [38]-[49].

The intraelement approaches are based on the concept of the strong discontinu- ity approach [50]–[56]. It can be shown that the introduction of strong discontinuity kinematics in a continuum medium, ruled by continuum (stress–strain) constitutive equations with strain softening, induces the fulfillment of specific traction–separation

constitutive laws at a discrete set of propagating cohesive surfaces [57]. These for- mulations allow the incorporation of a discontinuous mode on an element level, by exploiting the partition-of-unity property of the finite element shape functions [58].

A crack is modeled as a jump in the displacement field of the continuum elements, the magnitude of the jump is determined by an extra set of degrees of freedom, which are added to existing nodes of the finite element mesh. Remmers et al. [59] used this approach to formulate a solid-like shell element for the simulation of delamina- tion. However, the requirement of an extra set of degrees of freedom complicate the implementation of these formulations in commercial finite element codes.

Definition of the constitutive equation

The definition of the constitutive equation that relates tractions to displacement jumps at an interface can be done using a phenomenological or a mechanistic ap- proach.

The mechanistic approach to define the constitutive equation uses methods that derive directly the constitutive equation. There exist several methods in the litera- ture, using the direct tension test [60, 61], from measures using the J-integral and the final crack opening [62, 63] or using the fractal theory [64].

The phenomenological calibration of the constitutive equation is achieved using the results obtained in experimental tests. Constitutive equations are determined comparing the response of a test specimen (load-total displacement curve) with the results given with prediction models using different parameters. There are basically two groups of analysis to adjust the constitutive equation using experimental data [65]:

The first group are techniques that use a softening curve defined a prior by N parameters, which are best fitted by an optimization algorithm to the experimental data.

The second group uses characteristic points, or properties of the load-displacement curve (peak load or area under curve, for example). Several of such models have been

proposed. The simplest uses a bilinear constitutive equation [43]–[47]. In addition to the bilinear constitutive equation, there are different shapes of the constitutive equation formulated in the literature [34, 40, 43, 67] some of which are shown in Figure 2.8.

*Figure 2.8: Traction-relative displacement curves employed in various models in the*
*literature (Figure from Zou et al.[66]).*

Alfano [68] investigated the influence of the shape of the constitutive law compar- ing a bilinear, trapezoidal, exponential and linear–parabolic laws under static tests.

For a typical double-cantilever-beam test, the solution was found to be practically independent of the shape of the interface law. An influence of the interface law was found on the algorithmic numerical performance and on the degree of accuracy achieved; in particular, the trapezoidal law gave the worst results both in terms of numerical stability and in terms of convergence of the finite-element solution to the exact solution. The exponential law was found to be optimal in terms of accuracy while the bilinear law represented the best compromise between computational cost and accuracy.

## Chapter 3

## Variable mode-ratio interface damage model

### 3.1 Introduction

It was shown in the previous chapter that Cohesive Zone Models (CZM) are suit- able to simulate delamination because they can be used for both damage-tolerance and strength analysis. To become an eficient and robust design tool, the cohesive zone model formulation needs to predict the mode-ratio of crack propagation accu- rately. It is important to control the energy dissipation during delamination growth in order to avoid the restoration of the cohesive state, i.e., it is necessary to assure that the model satisfies the Clausius-Duhem inequality even while the mode-ratio changes during crack growth. There are several models in the literature that can be used under constant mode-ratio conditions [43, 45]-[47, 69]-[74]. However, the mod- els proposed generally do not satisfy the Clausius-Duhem inequality under variable mode loading. Most of the models cited above define the damage threshold param- eter as the maximum displacement. This assumption may lead to the violation of the Clausius-Duhem inequality when the crack grows in a varying mode.

The restoration of the cohesive state when the mode changes is illustrated in Fig- 39

*ure 3.1. This Figure represents the traction (τ )-relative displacement (∆) relation for*
*two different mode-ratios, G*_{II}*/ (G*_{II}*+ G*_{I}*) = A (Figure 3.1 a)) and G*_{II}*/ (G*_{II} *+ G*_{I}) =
*B (Figure 3.1 b)), where G*_{I}*and G*_{II} are the components of the energy release rate. If
the mode-ratio changes from A to B during delamination growth, there is a restora-
tion of the cohesive state. This effect is clearly inconsistent with the thermodynam-
ical principles.

### D

^{d}

### D t

### D t

Completely open

Delamination propagation Loading mode A

G /(_{II} G G_{II}+ )=A_{I}

Loading mode B
G /(G +G )=B_{II} _{II} _{I}

Restoration of the cohesive state

### D

^{d}

### t

_{A}

### t

_{B}

### t

_{A}

a) b)

*Figure 3.1: Restoration of the cohesive state for delamination propagation under*
*variable mode-ratio.*

A damage model for the simulation of delamination under variable mode is pre- sented in this thesis. A new delamination initiation criterion is proposed in order to ensure the consistency of energy dissipation rate under variable mode-ratio. The delamination onset criterion stems from the expression of the critical energy release rate for delamination propagation under mixed-mode loading proposed by Benzeg- gagh and Kenane [29].

This chapter is structured as follows: first, the formulation of the damage model for the simulation of delamination onset and growth model is presented. The finite

element discretization of the boundary value problem is described. Finally, the numerical predictions are compared with experimental results obtained in composite test specimens and composite structural components.

### 3.2 Model for delamination onset and propaga- tion

The boundary value problem, the kinematic equations, and the constitutive rela- tions are presented for the formulation of the model for delamination onset and delamination propagation.

### 3.2.1 Boundary value problem

Consider a domain Ω, as shown in Figure 3.2(a), containing a crack Γ*c*. The part
of the crack on which a cohesive law is active is denoted by Γ* _{coh}* and is called the
fracture process zone (FPZ).

W_{-}
W_{+}

G_{d}

G_{F}

G_{u}
G_{c}

G_{coh}
W

G_{F}

G_{u}

- +

(a) (b)

Figure 3.2: *Body Ω crossed by a material discontinuity Γ**d* *in the undeformed*
*configuration.*

*Prescribed tractions, t** _{i}*, are imposed on the boundary Γ

*, whereas prescribed displacements are imposed on Γ*

_{F}

_{u}*. The stress field inside the domain, σ*

*, is related*

_{ij}*to the external loading and the closing tractions τ*_{j}^{+}*, τ*_{j}* ^{−}*in the cohesive zone through
the equilibrium equations:

*σ*_{ij,j}*+ ρb** _{i}* = 0 in Ω (3.1)

*σ**ij**n**j* *= t**i* on Γ*F* (3.2)

*σ*_{ij}*n*^{+}_{j}*= τ*_{i}^{+} *= −τ*_{i}^{−}*= −σ*_{ij}*n*^{−}* _{j}* on Γ

*(3.3)*

_{coh}*where b*

_{i}*are the body forces, ρ is the density of the material, and n*

*is the vector normal to the surface.*

_{j}### 3.2.2 Kinematics of the interfacial surface

To develop the necessary kinematic relationships, consider the crack Γ* _{c}* shown in
Figure 3.2(a) as part of a material discontinuity, Γ

*, which divides the domain Ω into two parts, Ω*

_{d}^{+}and Ω

*(Figure 3.2(b)).*

^{−}The displacement jump across the material discontinuity Γ*d**, [[u**i*]], can be written
as:

*[[u**i**]] = u*^{+}_{i}*− u*^{−}* _{i}* (3.4)

*where u*^{±}* _{i}* denotes the displacement of the points on the surface of the material
discontinuity Γ

*d*of the parts Ω

*of the domain.*

^{±}The fundamental problem introduced by the interfacial surface Γ* _{d}* is how to
express the virtual displacement jumps associated to the surfaces Γ

_{d}*as a function of the virtual displacements. Consider a three-dimensional space with Cartesian*

^{±}*coordinates X*

_{i}*, i = 1, 2, 3 . Let the Cartesian coordinates x*

^{±}*describe the position of the upper and lower surfaces Γ*

_{i}

_{d}*in the deformed configuration. Considering Figure 3.3, any material point on Γ*

^{±}

_{d}*in the deformed configuration is related to its undeformed configuration through:*

^{±}Gd^{+}

Gd^{_}

G

d

v_{n}
P

P_

v_{t}
v_{s}
P_{+}

G = G_{d} _{d+}= G_{d-} =G_{d}
X_{3} X_{2}

X1

Deformed configuration Undeformed configuration

*u*_{i}^{+}_{+}

*u** _{-}*
h x

P =P+=P-

*Figure 3.3: Interfacial surface deformation.*

*x*^{±}_{i}*= X**i**+ u*^{±}* _{i}* (3.5)

*where u*^{±}* _{i}* are the displacements with respect to the fixed Cartesian coordinate sys-
tem. The coordinates ¯

*x*

*of the midsurface can be written as [76]:*

_{i}¯

*x*_{i}*= X** _{i}*+ 1
2

¡*u*^{+}_{i}*+ u*^{−}* _{i}* ¢

(3.6)
The components of the displacement jump vector are evaluated at the midsurface
Γ¯* _{d}*, which is coincident with Γ

*in the undeformed configuration (see Figure 3.3).*

_{d}*The midsurface coordinate gradients define the components of the two vectors, v**η**i*

*and v*_{ξ}* _{i}*, that define the tangential plane at a given point, ¯

*P :*

*v*_{η}* _{i}* = ¯

*x*

*(3.7)*

_{i,η}*v*_{ξ}* _{i}* = ¯

*x*

*(3.8)*

_{i,ξ}*where η, ξ are curvilinear coordinates on the surface ¯*Γ_{d}*. Although v*_{η}_{i}*and v*_{ξ}* _{i}* are
generally not orthogonal to each other, their vector product defines a surface normal.

Therefore, the local normal coordinate vector is obtained as:

v*n*= v*ξ**× v**η**kv**ξ**× v**η**k** ^{−1}* (3.9)

The tangential coordinates are then obtained as:

v* _{s}*= v

_{ξ}*kv*

_{ξ}*k*

*(3.10)*

^{−1}v* _{t}*= v

_{n}*× v*

*(3.11)*

_{s}The components of v_{n}*, v** _{s}* and v

*represent the direction cosines of the local coordinate system in the global coordinate system at a material point ¯*

_{t}*P ∈ ¯*Γ

*d*. The direction cosines define an orthogonal rotation tensor Θ

*relating the local coordinate system to the fixed coordinate system.*

_{mi}Using the rotation tensor, the normal and tangential components of the displace- ment jump tensor expressed in terms of the displacement field in global coordinates are:

∆* _{m}* = Θ

_{mi}*[[u*

*]] (3.12)*

_{i}where ∆* _{m}* is the displacement jump tensor in the local coordinate system.

### 3.2.3 Constitutive laws

*A constitutive law relating the cohesive tractions, τ** _{j}*, to the displacement jump
in the local coordinates, ∆

*, is required for modeling the behavior of the material discontinuity. The constitutive laws in the material discontinuity may be formally written as:*

_{i}*τ*_{j}*= τ (∆** _{i}*) (3.13)

*˙τ*_{j}*= D*^{tan}* _{ji}* ∆˙

*(3.14)*

_{i}*where D*_{ji}^{tan} is the constitutive tangent stiffness tensor.

A new constitutive model relating the displacement jumps to the tractions, and based on Damage Mechanics is proposed. The model follows the general formulation of Continuum Damage Models proposed by Simo and Ju [77, 78] and Mazars [79].

The free energy per unit surface of the interface is defined as:

*ψ (∆, d) = (1 − d) ψ*^{0}(∆) (3.15)

*where d is a scalar damage variable, and ψ*^{0} is a convex function in the displacement
jump space defined as:

*ψ*^{0}(∆) = 1

2∆*i**D*^{0}* _{ij}*∆

*j*

*i = 1, 3; j = 1, 3*(3.16) Negative values of ∆3do not have any physical meaning because interpenetration is prevented by contact. Therefore, a modification of Equation (3.15) is proposed to prevent interfacial penetration of the two adjacent layers after complete decohesion.

The expression for the free energy proposed is:

*ψ (∆, d) = (1 − d) ψ*^{0}(∆_{i}*) − dψ*^{0}*(δ*_{3i}*h−∆*_{3}*i)* (3.17)

*where h·i is the MacAuley bracket defined as hxi =* ^{1}_{2}*(x + |x|) and δ** _{ij}* is the Kro-
necker delta. The constitutive equation for the interface is obtained by differentiat-
ing the free energy with respect to the displacement jumps:

*τ** _{i}* =

*∂ψ*

*∂∆**i*

*= (1 − d) D*_{ij}^{0}∆_{j}*− dD*^{0}_{ij}*δ*_{3j}*h−∆*_{3}*i* (3.18)

*The undamaged stiffness tensor, D*^{0}* _{ij}*, is defined as:

*D*^{0}_{ij}*= δ*_{ij}*K* (3.19)